Published on Web 02/24/2004
Diamond and Diamond-Like Carbon from a Preceramic Polymer Patricia A. Bianconi,*,† Scott J. Joray,† Brian L. Aldrich,‡ Jitapa Sumranjit,† Daniel J. Duffy,† David P. Long,† Jason L. Lazorcik,† Louis Raboin,§ James K. Kearns,† Stephenie L. Smulligan,† and Jonathan M. Babyak† Contribution from the Departments of Chemistry and Polymer Science, UniVersity of Massachusetts at Amherst, Amherst, Massachusetts 01003, and Department of Chemistry, PennsylVania State UniVersity, UniVersity Park, PennsylVania 16803 Received October 27, 2003; E-mail: [email protected]
Abstract: The synthesis of poly(hydridocarbyne), one of a class of carbon-based random network polymers and a structural isomer of polyacetlyene, is reported. The network backbone of this polymer is primarily composed of tetrahedrally hybridized carbon atoms, each bearing one hydride substituent and linked via three carbon-carbon single bonds into a three-dimensional random network of fused rings. This atomiclevel carbon network backbone confers unusual properties on the polymer, including facile thermal decomposition to form diamond or diamond-like carbon high-quality films at atmospheric pressure, by direct deposition or by chemical vapor deposition (CVD), without the use of hydrogen or any other reagent.
A multitude of ways of fabricating diamond films by vapor deposition are known. All require a source of reactive hydrogen atoms, provided by hot filament, plasma, or microwave-assisted deposition. A drawback of these methods is that chemical vapor deposition (CVD) diamond films are not smooth or homogeneous enough to use in electronics or in coating for biomechanical devices such as MEMS; films must be machinepolished to attain the necessary smoothness. If highly sp3 diamond-like carbon (tetrahedral amorphous carbon) is deposited, to exploit these films’ smoothness and lubricity, their lack of purity limits their use; about 88% sp3 carbon is the greatest percentage reported for such materials. CVD is therefore not commercially feasible for many uses, especially for large-area projects. The preceramic polymer route to diamond films addresses these problems. Soluble polymer precursors may be cast, spun, or molded from the liquid phase, unlike any current diamond precursors, to form smooth films or conformal coatings. Pyrolysis or photolysis then converts the polymer film to a ceramic, the chemical formula of which is determined by the stoichiometry of the polymer backbone and side chains. An efficient preceramic polymer to diamond must be high in sp3 carbon, must contain hydrogen substituents to prevent conversion to sp2, and must have a high theoretical ceramic yield to obtain defect-free films. It was proposed when the †
Department of Chemistry, University of Massachusetts. Pennsylvania State University. § Department of Polymer Science, University of Massachusetts. ‡
10.1021/ja039254l CCC: $27.50 © 2004 American Chemical Society
synthesis and structure of polycarbynes were first reported,1 and has been confirmed by further research,1-12 that it is the unique sp3-hybridized, tetrahedrally bound carbon network backbone of this class of polymers that is responsible for their facile thermal and photolytic conversion to highly sp3 carbon ceramics at low pressures. The composition of the polymers has, however, been problematic: the polymer most easily synthesized and studied as a precursor to sp3 carbon is poly(phenylcarbyne), in which the phenyl groups substituted on the carbon network backbone give the polymer a 7:1 ratio of sp2/sp3 carbon. Thus, pyrolysis and photolysis carbon products of this polymer are composed of a high percentage of sp2 carbon.1,3-12 The optimum stoichiometry for a preceramic polymer to diamond is [CH]n, in which the sp3 network backbone is functionalized only with (1) Visscher. G. T.; Nesting, D. C.; Badding, J. V.; Bianconi, P. A. Science 1993, 260, 1496-1499. (2) Visscher. G. T.; Bianconi, P. A. J. Am. Chem. Soc. 1994, 116, 18051811. (3) Sun, Z.; Shi, X.; Tay, B. K.; Flynn, D.; Wang, X.; Zheng, Z.; Sun, Y. Diamond Relat. Mater. 1997, 6, 230-234. (4) Huang, S. M.; Lu, Y. F.; Sun, Z.; Luo, X. F. Surf. Coat. Technol. 2000, 125, 25-29. (5) Sun, Z.; Sun, Y.; Qihneg, Y.; Wang, X.; Zheng, Z. Surf. Coat. Technol. 1996, 75, 108-112. (6) Sun, Z.; Shi, X.; Tay, B. K.; Wang, X.; Zheng, Z. J. Mater. Sci. Lett. 1997, 16, 933-935. (7) Sun, Z.; Sun, Y.; Wlison, S. R. Thin Solid Films 2000, 377-378, 203207. (8) Sun, Z.; Zheng, Z.; Xun, Y.; Yang, Q.; He, Y. Thin Solid Films 1995, 257, 28-31. (9) Lu, Y. F.; Huang, S. M.; Sun, Z. J. Appl. Phys. 2000, 87, 945-951. (10) Huang, S. M.; Lu, Y. F.; Sun, Z. Jpn. J. Appl. Phys. 2000, 39, 11541159. (11) Wang, X.; Sun, Z.; Shi, X.; Chen, J.; Aheng, Z.; Yan, F. Mater. Sci. Eng., B 1998, 52, 216-219. (12) Sun, Z.; Shi, J. R.; Tay, B. K.; Lau, S. P. Diamond Relat. Mater. 2000, 9, 1979-1983. J. AM. CHEM. SOC. 2004, 126, 3191-3202
Bianconi et al.
hydrogen atoms; this “poly(hydridocarbyne)” would thus be a structural isomer of polyacetylene. We report here a synthetic procedure that leads to such a tractable, soluble, poly(hydridocarbyne) polymer product, and that, by thermolysis, this preceramic polymer converts to diamond and sp3 carbon in very high yields. Experimental Section General Procedures. All the reactions were carried out under a nitrogen or argon atmosphere, by means of standard Schlenk manipulations or inside a glovebox. Anhydrous pentane, dimethoxyethane, and tetrahydrofuran were purchased from Aldrich and were dried over sodium metal and benzophenone and distilled prior to their use. Bromoform (99%) was purchased from VWR and used as received. Methyllithium (1.4 M in diethyl ether) was purchased from Aldrich and used as received and later titrated to correct the concentration. Liquid 1:1 mole ratio NaK alloy was prepared in a glovebox by adding solid potassium to an equimolar amount of molten sodium. Caution! NaK alloy is pyrophoric and can be explosiVely reactiVe, especially with water and halocarbons. Handle with all necessary precautions and in inert atmospheres only. Elemental analyses were performed at the Microanalysis Laboratory, University of Massachusetts, Amherst, using V2O5 as a combustion aid. 1H NMR (200.1 MHz) spectra were recorded on a Bruker AC200, and 13C NMR (75.5 MHz) spectra were recorded on an Avance DSX300 instrument. FTIR transmission spectra were obtained using a Midac M12-SP3 spectrometer, operating at 4 cm-1 resolution. Electronic spectra were measured using a Shimadzu UV-260 spectrometer. Raman spectroscopy was performed on a Bruker FRA-106 with a Nd:YAG laser at 1064 cm-1 and a JY Horiba LabRam HR800 micro Raman spectrograph operating at 785 nm. Microfocus visible Raman spectra were acquired on Kaiser Hololab 5000R Raman spectrometer utilizing a coherent continuous wave Ar ion laser operating at 514 nm. UV Raman spectra at 257 nm were collected with a single stage of a model 1400 SPEX spectrometer equipped with a Princeton Instruments model 1340-PB backthinned charge-coupled device (CCD) detector. A Coherent FRED frequency-doubled argon ion laser was used for excitation at 257 nm. After passing through a Pellin-Broca prism and spatial filter, the laser light was focused at an angle of 35° onto the sample with a spot size of approximately 10 µm. The scattered light was collected with a Coherent Ealing 0.5 NA 15 reflecting objective. The Rayleigh scattered light was rejected by a pair of Omega Optical dielectric edge filters. UV Raman spectra at 244 nm were acquired on a Spectra-Physics BeamLok 2060-7s argon ion laser whose 488 nm emission was frequency-doubled to 244 nm by the Spectra-Physic Wavetrain which uses a BBO crystal for SHG, with 0.8 mW power and an acquisition time of 30 s. UV Raman spectra at 229 nm were collected using two Renishaw microRaman 1000 spectrometers on a 40× objective, with a UV-enhanced CCD camera, with 0.3 mW of power. The carbon films were treated immediately prior to the acquisition of Raman spectra by exposure to oxygen plasma (19 mW, 5 min, room temperature) to remove surface layers of adventitious C-H material, which is readily adsorbed by the films, and to avoid spurious signals in the spectra.13 Dynamic light scattering was performed at room temperature on an ALV instrument with an ALV5000e correlator and an argon ion laser (514 nm). Size exclusion chromatography was run at 120 °C in DMSO on a Polymer Laboratories (Amherst, MA) PL220 GPC system with RI detector and a Wyatt (Santa Barbara, CA) high-temperature miniDAWN light scattering detector. ESR spectra were recorded on an ESP-300 electron spin resonance spectrometer (IBM Instruments Inc.). Pyrolysis studies were performed using a Thermolyne 12110 tube furnace, with samples placed in a ceramic boat. Polymer films were (13) Knight, D. W.; Weimer, L. P.; White, W. B. Appl. Phys. Lett. 1990, 56, 1320-1322. 3192 J. AM. CHEM. SOC.
VOL. 126, NO. 10, 2004
spun using a Headway Research, Inc. Photo Resist spinner model 1-EC101DT-435, from a 0.2 g/mL polymer/THF solution. Film thickness and roughness measurements were obtained using a Tencor Instruments Alpha Step 500 surface profiler. Field emission scanning electron microscopy (FE-SEM) and energy-dispersive X-ray spectroscopy (EDS) were carried out a JEOL JSM-6320 FXV field emission scanning electron micrograph. The XRD patterns were recorded on a Siemens D-500 diffractometer in transmission geometry with Ni-filtered Cu KR radiation. Atomic force microscopy was performed on a NanoScope IIIa scanning probe microscope (Digital Instruments). A JEOL 100CX scanning transmission electron microscope, equipped with an IMIX-XE PGT detector digital spectrometer (Princeton GammaTech), was used for transmission electron microscopy and energy dispersive spectroscopy. X-ray photoelectron spectroscopy was performed on an ESCA 8502A, version 2.0 C instrument (Perkin-Elmer Physical Electronics Division). Synthesis of Poly(hydridocarbyne) (1). An oven-dried 600-mL beaker was placed in a nitrogen atmosphere drybox equipped with a high-intensity (475 W, 20 kHz, 1/2 in. tip) ultrasonic immersion horn and was charged with THF (200 mL), anhydrous dimethoxyethane (10 mL), and sodium potassium alloy (NaK, 2.33 g, 37.5 mmol). The ultrasonic horn was immersed in the reaction mixture to a depth of 1 in. above the bottom of the beaker, and the solvents and NaK were irradiated at 17% power output for 5 min, producing a blue emulsion. Bromoform (6.32 g, 25 mmol) was diluted with 40 mL of THF and was added to the NaK emulsion dropwise over approximately 12 min, while being sonicated as before. During the addition, the reaction mixture heated to reflux; care was taken to control the vigor of the reaction by controlling the rate of addition of the remaining bromoform. The emulsion became dark brown upon addition of the bromoform and turned black by the end of the addition. After the addition was complete, sonication was continued for approximately 18 min. The black reaction mixture was allowed to cool and was then transferred to a shielded fume hood under ambient atmosphere. Water (5 mL) was added to the reaction mixture to quench any unreacted NaK. The solution was then decanted from white salts that had precipitated upon the addition of water, and the solvents were evaporated under vacuum. A dark brown waxy solid, combined with a white band of salts, remained. Dichloromethane (10 mL) was added, forming a dark solution with a white salt precipitate. The solution was decanted from the salts and was reduced in volume by half; hexanes (approximately 15 mL) were gradually added until a fine tan to brown precipitate of poly(hydridocarbyne), 1, formed, which was gravity-filtered and air-dried. The polymer was typically obtained as a fine brown powder in yields of 0.15-0.28 g (46-85%). Additional polymer could be recovered by evaporating the filtrate solution to dryness, redissolving the solids in minimum dichloromethane, and precipitating with hexanes as before. 1 H NMR (CDCl3): δ 1.0-3.0 (weak, CH), 1.59, 1.25 (C-CH3). 13C CPMAS NMR: δ 15 (CCH3), 30.08 (aliphatic CH), 50-100 (broad, CBr), 114.8 (vinylic CH, cis), 138 (vinylic CH, trans). IR (THF solution, cm-) 2975 (s), 2874 (s), 2858 (s), 1458 (m), 1365 (w), 1180 (w), 1068 (vs), 911 (s), 657 (w). Anal. Calcd for (CH): C, 92.31; H, 7.69. Found: C, 65.34-70.42; H, 7.71-8.21; Br,